utilization of constructional lime as heterogeneous ... original paper utilization of constructional
Post on 27-Aug-2019
Embed Size (px)
Utilization of constructional lime as heterogeneous catalyst in biodiesel production from waste frying oil
R. Ghanei • G. Moradi • A. Heydarinasab •
A. A. Seifkordi • M. Ardjmand
Received: 24 January 2012 / Accepted: 2 August 2012 / Published online: 19 March 2013
� Islamic Azad University (IAU) 2013
Abstract Waste frying oil as valueless material which is
disposed to environment can be used as a promising
feedstock to produce biodiesel. In this study, constructional
lime was used as alkaline heterogeneous catalyst for bio-
diesel production from virgin and waste frying oil. After
determining the best activation temperature for the catalyst
(600 �C), transesterification reactions were carried out at 65 �C, MeOH to oil molar ratio of 12:1, and 1 wt% of activated constructional lime under vigorous mixing for
5 h. Yield of reactions for virgin and waste frying oil
(2.17 % free fatty acid) and pretreated waste frying oil
(0.918 % free fatty acid) were 87, 93.9, and 94 %,
respectively. Transesterification of virgin frying oil and
pretreated waste frying oil were done at 65 �C, MeOH to oil molar ratio of 6:1, and 1 wt% of KOH as catalyst under
vigorous mixing for 2 h, for comparison. Yield of the
reaction was 98.6 and 95.1 %, respectively. Therefore,
when constructional lime is used as catalyst pretreatment of
waste oil is not necessary.
Keywords Fatty acid methyl ester � Lime � Solid base catalyst � Transesterification � Waste oil
Fatty acid alkyl ester (FAAE) or biodiesel which is pro-
duced from renewable feed stocks such as vegetable oils
and animal fats has gained great attention of many nations
in recent decade. This bio-fuel is a sustainable alternative
for decreasing fossil diesel, and will be very important in
future (Janaun and Ellis 2010; Jacobson et al. 2008; Umdu
et al. 2009; Zabeti et al. 2009a; Silva et al. 2010). More-
over, it has a lot of benefits rather than traditional diesel
fuel. Some of them are as follow: environmental friendly
emissions, biodegradable and renewable, non-toxic, better
lubricity, no sulfur, and aromatic content, and it can be
used in diesel engine without any change (Jacobson et al.
2008; Umdu et al. 2009; Leung et al. 2010; Li et al. 2009;
Ghanei et al. 2011; Balat and Balat 2010). Furthermore, it
is the only alternative fuel that passed the health effects
testing requirements of the 1990 Clean Air Act Amend-
ments (Jacobson et al. 2008).
Biodiesel is produced by alcoholysis (commonly meth-
anolysis) of triglycerides (TGs) in the presence of appro-
priate catalyst. This reaction is called as transesterification.
Figure 1 shows the scheme of the mentioned reaction
(Leung et al. 2010; Ghanei et al. 2011; Veljković et al.
2009, Boz et al. 2009; Helwani et al. 2009). Since the cost
of raw material has a major impact on final price of bio-
diesel, use of inexpensive feed stocks such as waste frying
(WFO) and cooking oil (WCO) is recommended to reduce
final price of biodiesel. The main problem of these type oils
is high free fatty acid (FFA) content which makes some
difficulties in process (Jacobson et al. 2008; Fraile et al.
Electronic supplementary material The online version of this article (doi:10.1007/s13762-012-0137-4) contains supplementary material, which is available to authorized users.
R. Ghanei (&) � A. Heydarinasab � A. A. Seifkordi Department of Chemical Engineering, Science and Research
branch, Islamic Azad University, Tehran, Iran
Department of Chemical Engineering, Engineering Faculty,
Razi University, Kermanshah, Iran
Department of Chemical Engineering, Tehran South branch,
Islamic Azad University, Tehran, Iran
Int. J. Environ. Sci. Technol. (2013) 10:847–854
2009; Sharma and Singh 2009; Sabudak and Yildiz 2010).
Although strong and homogenous bases are able to
accomplish the reaction over 98 %, very fast recovery of
catalysts is much difficult and makes hazardous waste
waters (Ghanei et al. 2011; Veljković et al. 2009; Kawa-
shima et al. 2008; Silva et al. 2010). Moreover, when waste
oils are used as feed, the catalyst is consumed to form soap
instead of biodiesel due to the high FFA of used oil
(Jacobson et al. 2008; Ghanei et al. 2011; Balat and Balat
2010). Hence, introducing new catalytic systems, espe-
cially heterogeneous catalysts, is necessary. Heterogeneous
catalysts are separated from products easily and they can be
used several time, and also prevent the formation of
unwanted byproduct and waste waters (Li et al. 2009;
Ghanei et al. 2011; Kawashima et al. 2008; Boz et al. 2009;
Guo et al. 2010).
There are two main categories in heterogeneous cata-
lysts that are applicable in transesterification process,
acidic and basic solids. In the first group solid acids such
as tungstophosphoric acid, zinc ethanoate, zinc stearate
and transition metal oxides which have acidic character-
ization on alumina and silica as support were investigated,
and zinc stearate on silica gel selected as the best one
(Jacobson et al. 2008; Helwani et al. 2009; Sharma and
Singh 2009). In the second group, further investigations
have been performed due to good accessibility and high
activity in moderate reaction conditions. Alkali earth
metal oxide and methoxide and mixture of them, espe-
cially calcium oxide, are reported as active catalysts
(Veljković et al. 2009; Kawashima et al. 2008; Sun et al.
2010; Liu et al. 2007; Wen et al. 2010; Liu et al. 2008a,
2008b; Zabeti et al. 2009b; Fraile et al. 2009; Guo et al.
2010). In most cases, laboratory grade or synthesized
CaO, which is expensive, with or without support has
been used as catalyst to transesterify the virgin edible oil
to biodiesel, and high yield has been achieved (Liu et al.
2008b; Kouzu et al. 2008, 2009; Albuquerque et al.
2008). Recently, in order to prepare CaO from low
expense and useless resources, use of waste materials
such as egg shell, oyster shell, mud carb shell, and cockle
shell has been reported by Chakraborty et al. (2010),
Viriya-empikul et al. (2010), Nakatani et al. (2009) and
Boey et al. (2009, 2011), respectively.
Lime as a constructional material is produced from
heating of lime stone in the large traditional limekiln, in
commercial scale. Calcium oxide is the predominant con-
stituent of lime that absorbs water intensively and forms
quicklime (calcium hydroxide). Thus, this inexpensive and
abundant material can play the role of catalyst in transe-
sterification of vegetable oils, with a minor pretreatment.
Low price of constructional lime (CL) and WFO, and lack
of sufficient information in this field encouraged us to
perform this work. In the present study, transesterification
of virgin and WFO in the presence of lime as catalyst have
been investigated. In the first step, appropriate temperature
for catalyst pretreatment process was determined. Then,
transesterification of WFO with and without acid pre-
treatment were performed, and the products were evalu-
ated. Finally, the results were compared to corresponding
homogenous alkali catalyst process. The main steps of
research were done during 2011 in Biodiesel Research
laboratory of Islamic Azad University (Farahan branch),
Farahan, Iran. Also some analytical services were received
from Isfahan University, Isfahan, Mahidasht agro-industry,
Kermanshah, and NPC-RT co., Tehran, Iran.
Materials and methods
Waste frying oil was collected from local restaurant. Virgin
frying oil (VFO) with the brand name of ‘‘Varamin’’ was
supplied by the mentioned restaurant. Constructional lime
was supplied from construction workshop in campus. The
reagents used during synthesis and purification procedures
were: methanol 99.9 % (chromatography grade, Merck),
potassium hydroxide (KOH) 85 % pellets (GR for analysis,
Merck), hydrochloric acid 37 % (GR for analysis, Merk),
n-Hexane 95 % (extra pure, Merk), and some other
chemicals were purchased from country company. Methyl
laurate (methyl dodecanoate) C99.7 % were supplied from
Sigma as standard for GC analysis.
Excess amount of lime was charged in a crucible and it was
put in electrical furnace. The furnace was warmed up to the
Fig. 1 The scheme of transesterification of
848 Int. J. Environ. Sci. Technol. (2013) 10:847–854
assigned temperature and this condition was kept for 4 h.
Then, activated catalyst was cooled to 150 �C, naturally. At this time, appropriate amount of catalyst was weighed
and transferred to reactor, immediately.
The X-ray diffraction (XRD) pattern